Mechanical Properties of Hydrocolloid and Rubber Impression Materials
Hampson' has studied the elasticity of alginates under compression and has observed that materials with smaller amounts of permanent deformation were more suitable for use in the presence of undercut areas. Schoonover and Dickson2 report the breaking stress, percent strain, and percent set of alginates. Cresson3 suggested the revision of the testing procedure for compressive strengths of dental elastic impression materials that would apply the load at the rate of 18,000 Gm. per minute. Skinner et al.4 and Phillips5 point out the importance of the rate of deformation on the technic of handling alginate hydrocolloids. Warner" also shows that the breaking strength and percent deformation of alginates are functions of the loading rate where the higher the rate, the greater is the strength qualities. Anderson7 shows the recovery from deformation of alginate to be a direct function of time from the start of mixing. Donnison and Docking8 have measured the permanent deformation, stiffness, and toughness of alginates, the latter being determined as a combination of compressive strength and the strain at rupture. The ADA Specification 189 requires the compressive strength to be determined at a rate of 10,000 -+ 2 000 Gm. per minute. Based on an average strength of 7,000 Gm./cm.2 and a specimen '2 inch in diameter, the time required for rupture would be approximately half a minute. Recently, Braden'0 has determined the energy of tearing of one each of mercaptan, silicone, and alginate impression materials as a function of the rate of tearing and the temperature of testing. As the rate of tearing increased and the temperature decreased,
Effect of sodium fluoride addition as a disinfectant on some properties of alginate impression material
Impression materials, impression trays, and poured stone cast have been said to be the main source of cross infection between patients and dentists. However, it was observed that disinfection of the impression is not performed systematically in routine dental practice. Disinfection of alginates either by immersion or spray technique was found to cause dimensional inaccuracies, although with proper disinfection of alginates there were small dimensional changes. A variety of fluoride releasing products designed for topical use is currently available. Following their use, varied amount of fluoride is systemically absorbed depending on the fluoride concentration and the manner of its use. The objective of this study was to evaluate the effect of addition (0%, 0.25%,0.5%,1%, 2%, 3%, 4% ) of (NaF) as a self-disinfection to alginate impression material powder and its effect on setting time, tear strength, dimensional change and accuracy of alginate impression materials. Materials and methods: A total No. of (700) specimen were used in this study.These specimens were divided into (5) main groups according to the tests used. Each of the four main groups contain (70) specimen divided into 7 subgroups (ten specimens to be tested for each (7)concentrations which is composed of six percentages of NaFwith alginate powder (0.25%,0.5%,1%, 2%, 3%, 4% )and one for control (0% NaF) , while the fifth group (Microbiological test) contain 420 specimen were divided between Streptococcus mutans and Candida albicans as (120) specimen for each one that was subdivided into three subgroups (specimens taken before impression casting, specimensafter pouring of alginate with stone andspecimens of stone were taken from the casts) in which it contain the same subgroups of the other concentrationsof (NaF) to test its efficacy against (Streptococcus mutans and Candida albicans). Results: Tear strength for all experimental impression materials was greater than those of the control products. There were no statistically significant differences between the dimensional change tests and also reproduction of detail test.With regard to setting time of the impressions, statisticallyreduction were seen between the control and experimental groups of alginate impression materials that contain (NaF). Self-disinfection of alginate impression material containing NaF showed a significant reduction in the count of cell forming unit of microorganism s immediately after impressions were made. Conclusion: In cooperation of specific concentrations of (NaF) as a disinfectant in alginate dental impression produced a significant reduction of contamination, also they caused non-significant effect on dimensional stability, detail reproduction and significant increase in tear strength. Therefore it is recommended as step in preventing cross
Dimensional stability of alginate impression materials.
Introduction: In 2001, Cavex presented the first test results, which showed 5 days dimensional stability for Cavex ColorChange. More than 10 years we used this information to show our customers the high quality and stability of our products. In the meantime, our Research & Development department worked on improvements of the alginate impression materials. We formed close cooperation’s with suppliers to understand more the chemistry of the used ingredients and discussed the important characteristics of alginate impression materials with our dealers all over the world. As a result, slight improvements were obtained for the Cavex alginates. In 2010, we launched a project together with the department Dental Material Science of ACTA (University of Amsterdam). Goal was to make a total evaluation of 6 major brands of alginate impression materials (CAVEX CA37, JELTRATE, AROMA FINE, HYDROGUM, KROMOPAN, COLORCHANGE). The main topics of the research were defined: dimensional stability, compressive strength, density, acidity (pH)